IS 9417 : 1989
yr REINFORCEDCONCRETECONSTRUCTION-ICd RECOMMENDATIONSFORWELDING
( First Revision)
UDC 669’14-422-131’2 : 621’791 : 693’55
@ BIS l&O
BUREAU OF INDIAN STANDARDS
MANAK BHAVAN, 9 BAHADUR SHAH ZAFAR MARG
NEW DELHI 110002
January 1990 Price Group 4
( Reaffirmed 1994 )
Welding Application Sectional Committee, SMDC 15
This Indian Standard ( First Revision ) was adopted by the Bureau of Indian Standards on
13 February 1989, after the draft finalized by the Welding Application Sectional Committee had
been approved by the Structural and Metals Division Council.
This standard was first published in 1977, deriving assistance from DIN 4099 ( Part 1 )-1972
‘Welding of reinforcing steel - Requirements and tests’, issued by the Deutsches Institut
fur Normung and keeping in view the practices prevailing in the conutry at that time.
In view of the experience gained over the years in the welding of cold-worked steel bars, the
Committee has revised this standard by effecting the following major modifications:
a) Resistance but welding of cold-worked bars has been deleted since it is no longer in use.
b) A reference to gas pressure welding of cold-worked bars has been made. This technique
although being extensively used in some foreign countries, is relatively new and yet to be
commercially used in India.
This standard incorporates the provisions for the welding of cold-worked steel bars conforming to
Grade Fe 415 and Fe 500 of IS 1786 : 1985. For welding micro alloyed steel bars, a reference
may be made to IS 9595 : 1980 in regard to the provisions relating to carbon equivalent establish-
ing welding procedures and other relevant details.
For the welding of thermo-mechanically treated bars, the provisions would be covered at a later
date on necessary experience and data becoming available.
Provisions for welding of mild steel bars for reinforced concrete construction have been covered in
IS 2751 : 1979.
IS 9417 : 1989
WELDING - COLD-WORKED STEEL BARS FOR
REINFORCED CONCRETE CONS‘TRUCTION -
RECOMMENDATIONS FOR WELDING
( First Revision )
1.1 This standard lays down recommendations
for welding cold-worked steel bars conforming
to Grade Fe 415 and Fe 500 of IS 1786 : 1985
‘Specification for high strength deformed steel
bars and wires for concrete reinforcements
( rhird retision )’ by flash butt welding, shielded
metal arc welding and gas pressure welding
2.1 The lndian Standards listed in Annex A are
necessary adjuncts to this standard.
3.1 For the purpose of this standard, definitions
given in 1s 812 : 1957 shall apply.
4 PLANS AND DRAWING
4.1 Plans and drawing for welding reinforced
steel bars shall be prepared in accordance
with SP 46 : 1988.
5.1 Symbols for welding used in plans and shop
drawings shall conform to IS 813 : 1986.
6 WELDING EQIJIPMENT AND
6.1 Welding equipment and accessories used in
welding of steel bars for concrete reinforcement
shall conform to the requirements of the appro-
priate Indian Standards where available. Where
an Indian Standard is not available, equipment
and accessories shall be of the best available
quality. Their capacity shall be adequate for
the welding procedure. A general guidance for
selection of equipment and accessories is includ-
ed in Annex B.
7 PARENT METAL
7.1 The parent metal shall be of guaranteed
weldable quality of steel conforming to IS 1786 :
8 SAFETY AND HEALTH REQUIREMENTS
8.1 Safety and health requirements as prescribed
in IS 818 : 1968 shall be applicable. Fire pre-
cautions shall be as given in 1S 3016 : 1982.
9.1 Electrodes used shall conform to 1S 814
(Part 1 ) : 1974.
10 WELDING PROCESSES AND
10.1.1 Cold-worked steel bars shall be either
butt welded or lap welded. Butt welding may
be carried out either by flash butt, gas pressure
or by shielded metal arc welding process. Lap
welding may be carried out by shielded metal
arc welding process.
10.1.2 Bars of unequal diameter may be welded.
However, in case of butt welding, the difference
in, diameter of bars shall not exceed 5 mm.
Where unequal diameter bars are welded, the
dimension ‘Ct’mentioned in this standard refers
to the diameter of the smaller bar.
10.1.3 The untwisted ends must be removed
before welding and the surface of the ends of the
bars to be welded shall be clean and free from
rust, paint, grease and/or other contaminants
which are likely to affect the quality 01 weld.
10.2 Flash Butt Welding of Cold-Worked Bars
Flash butt welding may be adopted if a large
number of welding has to be done at the same
place and when the electric supply is available
of the required capacity in respect of the cross
sectional arca of the maximum size of the bar
to be welded.
10.2.2.1 The ends of the bars to be welded
should be placed in proper alignment in clamps
so that bent or ccccntric joints do not result.
The clamps should bc clcancd bcforc each weld-
ing operation to avoid current loss and to
eliminate harmful notches or grooves due to
burning in of spots of arcing.
10.2.2.2 The bar ends shall bc unjformly pushed
against each other from the moment of contact
to the up-setting. The transfoi-mcr regulator
should ‘bc SO set that thi: cui~rcnt :tt 1hc contact
arca is bctwecn 85 to 90 A/mml.
10.2.2.3 If the capacity of butt welding machine
or the available power is not sufficient to take
the load for welding from cold, welding may be
done after preheating. By making and breaking
of the contact arc repeatedly, heat can be made
to spread over the entire cross section of the
bar. The number of short-circuits ( contacts
and reversing > should be kept to the minimum
possible so that the welding time and spread of
heat in the longitudinal direction in the bar is
minimum. Satisfactory joints with only slight
reduction in original strength of the bar can be
achieved with a current density up to 25 A/mm’.
10.2.2.4 In automatic machines, the flash rate
should be so set that a continuous flash without
interruption can be achieved. If the rate is set,
too high additional short-circuits are required
leading to heat spread. If the rate is too low,
the flash will be interrupted and consequently
air penetrating into the joints will form oxides.
If the machine is hand-operated, the flash should
be maintained to avoid interruption. Too long
flashes lead to generation of large quantities of
heat thus removing the effect of cold-working in
10.2.2.5 For bars with sheared ends, a burn-off
( flash-off) length of about 5 to 7 mm is requir-
ed (this length is practically independent of the
bar diameter >. Very short burn-off lengths
lead to defective welding because all the impuri-
ties may not have been removed from the place
of welding. Increase in the burn-off length
will spread heat along the length of the bar
thus reducing the strength of the bar.
10.2.2.6 The up-setting should result from the
burning off, that is, without interruption in the
rain of sparks. The electric supply should be
switched off about l/3 to 1 second after the start
of the up-setting or in the case of automatic
machine after 1 to 3 mm of up-set travel.
The voltage and frequency of the current should
be checked before commencing the welding
operation. Deviations from the nominal value
or large fluctuations during the operation may
lead to gross defects in welding. Wherever pos-
sible, welding should be done during day time
when the total load on the network is fairly
10.3 Butt-Welding by Shielded Metal Arc
Butt-welds by metal arc welding process are
normally adopted to join bars of thickness more
than 20 mm.
10.3.2 Preparation for Welding
10.3.2.1 The preparation of the edges of the
rods shall be as shown in Fig 1. The edges shall
be prepared by shearing, machining, or oxy-
acetylene flame cutting. Bevelling may be made
by machining, grinding oxy-acetylene cutting.
The fusion faces and the surrounding material
shall be free from scale, dirt, greases, paint, rust
10.3.2.2 When it is not possible to rotate the
bars for carrying out all welding in flat position,
the edge preparation shall be such that welding
is done on both sides in the vertical position.
10.3.2.3 All the bars to be butt welded should
be aligned and set up in position with their axis
in one straight line. This may be done in a jig
or by means of a clamp or by using guides.
Rotation of the bars should be avoided until
they are adequately welded so that no distur-
bance to the alignment is caused and no twist is
introduced in the bars during the process of
welding. The joints may not be out of align-
ment by more than 25 percent of the thickness
of the thinner material for material up to and
including 12 mm thick, or by more than 3 mm
for thicker material.
10.3.3.1 Welding electrodes with flux covering
of Type 3 or Type 6 of IS 815 : 1974 ara
YFUSION FACES CLEANEG
FIG. 1 EDGE PREPARATION
recommended for better results depending
on the size of the bar to be welded. Storage of
the latter type and their drying immediately
prior to use must be strictly in accordance with
the recommendation of the electrode manufac-
10.3.3.2 The size of electrodes depends upon the
position of the bead and thickness of the bar to
be welded. The root runs should be made
with electrodes of size not exceeding 2’5 mm.
For successive beads, the size of the electrodes
should be progressively increased so that in the
top bead, the electrode size does not generally
exceed 3’15 mm for 20 mm bars and 5 mm for
40 mm bars.
10.3.3.3 Concentration of heat shall be avoided
by proper welding sequence and manipulation of
10.3.4.1 The sequence of welding beads is shown
in Fig. 2. The runs 1 to 4 are made in the
position of welding best suited for the quality
of the weld. Besides the interruption in weld-
ing required for cleaning of each bead, a pause
shall be made after every second bead and the
bar is allowed to cool. The temperature of the
bars at a distance of about one bar diameter
from the joints shall not exceed 300°C immedia-
tely after the bead is made. Before commencing
the next bead, the temperature shall not exceed
250°C. The temperature may be checked approxi-
mately by using temperature indicating cray-
ons. However, in the absence of temperature
indicating devices, the bar may be allowed to
cool down to handhot temperature before the
next bead is deposited.
After completing bead 4, the bars are turned
through 180” and the beads 5 to 7 are made in
the same manner as described above. The top
bead 8 is deposited as the joint is continuously
rotated and the size of the reinforcement should
be approximately as indicated in Fig. 2.
IS 9417: 1989
10.3.4.2 In the case of non-rotatable bars, the
beads 1 to 4 should be made as explained in
10.3.4.1. The welder then moves to the other
side and beads 5 to 7 are similarly made. It is
difficult to deposit a uniform top bead for non-
rotatable bars and it may be necessary to make
two or more separate annular runs so that the
joint is approximately axisymmetric and has
sufficient reinforcement as shown in Fig. 2.
10.4 Butt Welding by Gas Pressure Welding
10.4.1 Gas pressure welding is basically a hot
forging process of joining the two bars end to
end. The bar ends are heated by a multi-nozzle
burner using oxy-acetylene flame and fused by
forcing the two bar ends against each other
under pressure to effect a solid phase welded
10.4.2 Recommendations in regard to the pre-
paration for welding procedure and equipment
are given in Annex C.
10.5 Lap Weldiug of Cold-Worked Bars
Lap joints may be made in cold-worked bars of
all sizes. They are preferred when access for
welding is from one side only, and while con-
necting prefabricated units. Use of electrodes
with flux covering of Type 3 or Type 6 of
IS 815 : 1974 are recommended for better results
depending on the size of bar being welded.
Storage of the latter type and their drying im-
mediately prior to use must be strictly in accor-
dance with the recommendations of the electrode
10.5.2 Preparation for Welding
Edge preparation is not necessary for lap welds.
The joint faces and the surrounding material
shall be free from scale, dirt, grease, paint, rust
FIG. 2 SEQUENCEOFWELDING
IS 9417: 1989
The size of electrodes according to the diameter
of the bar to be welded shall be as follows:
Nomin;loX;meter of Size of Electrode,
Up to and including 10 2’5
Over 10 up to and 3’15
Over 18 up to and 4’0
Over 28 5’0
The arc should be struck as shown in Fig. 3
“7STRIKING Of ARC - wlTHDRAWnL
somewhere in the middle of the joint and not
at its beginning.
The movement of the electrode for welding lap
joints in the horizontal and vertical position is
indicated in Fig. 3.
The various lap joints used to connect cold-
worked bars are shown in Fig. 4 to 7.
In Fig. 4 to 6, the dimensions indicated as ‘5d’
for single side welding should be halved to ‘2’5d’
if the welds are deposited from the opposite side
also. The single-strap arrangement shown in
Fig. 7 is not recommended where access is from
one side only. In the case of joints illustrated
in Fig. 6 and 7, the strap material must also
conform to 7 and the strap cross sectional area
must, at least, equal that of the bar to be joined.
32 WELDING IN THE HORIZON~AC
3b wE1_Dlt4G IN THE
FIG. 3 WELDING OF LAP JOINTS
1. Strike the electrode here; the arc striking point must lie in the groove which will be subsequently
2. Welding directions for horizontal or near-horizontal lap joints; in the case of vertical Jar, joints,
the welding shall be performed from bottom to top ( rising 1.
3. Lift-oK electrode.
FIG. 4 LAP JOINT
FIG. 5 LAP JOINT ( VARIANT )
IS 9417: 1989
1. Strike the electrode here; the arc striking point must lie in the groove which will be subsequently
2. Welding directions for horizontal or near-horizontal strapped joints; in the case of vertical strapped
joints, the welding shall be performed from bottom to top ( rising ).
3. Lift-off electrode.
4. Butted bar.
FIG. 6 STRAPPED JOINT ( ~=NOMINAL DIAMETER OF BUTTED BAR )
GAP 2 T03mm--cj
FIG. 7 STRAPPED JOINT ( VARIANT )
11 VISUAL INSPECTION
Each welded joint shall be visually inspected for
11.1 Sbape of Profile
The profile of the welds shall be uniform, slight-
ly convex and free from overlap at the toes of
11.2 Uniformity of Surface
The weld surface shall be uniform in appearance
throughout its length and shall show no
pronounced hump or crater.
31.3 Degree of Undercut
conditions to establish that the proposed joints
can be made satisfactorily. For the purpose,
the tests shall be the same as for ‘Quality Cont-
rol Tests’ in 13 but only 3 test pieces will be
required for tensile test and 3 for bend test.
Such initial tests shall be repeated if there is any
a) the welding process;
b) the grade of cold-worked steel bars;
c) the type or size of electrode;
d) the welder; and
e) the position of welding, unless the new
position is an easier one.
The welded joint shall be free from undercut
but slight intermittent occurrences may be dis-
13 QUALITY CONTROL TESTS
Il.4 Freedom from Surface Defects
13.1 Butt Welds
The surface of the weld shall be free from cracks, TCSt pieces containing butt welds at the
cavities, solid inclusions and other visible centre in the as-welded condition shall be select-
ed at the rate of one for tensile test and one
for bend test for evcrv 100 ioints or as decided
The misalignment of the bars welded shall not
exceed one-fourth of bar diameter or 5 mm
whichever is less.
NOTE - Misalignment shall be evaluated on the
basis of smaller diameter in c:lse of bars of unequal
diameters are used.
12 INITIAL TESTS
12.1 Prior to production welding, test welds
shall be carried out under the local production
by the engineer-in-ci;arge. _I
Unm:~chineil specimens with a free length bet-
ween grips about 20tl should he used. The
sclccted pieces when sub_jccted to :t tensile test
shall have tcnsilo strenglh not less than 90 per-
cent or the actual tensile strength of the bar but
in no case less than 485 MPa for grade Fc 415
and 545 MPa for grndc Fe 500 of IS 1786 : 1985.
The fracture shall not take place in the weld
IS 9417 : 1989
13.1.2 Bend Test
The welding flash or reinforcement shall be
removed at the point where contact is made
with the mandrel. The welded joint shall be
capable of being bent to an angle of 60’ around
a mandrel of diameter specified below, before
any crack appears:
IVominal Diameter of Diameter of Mandrel
up to 10 5d
Over 10 Id
13.2 Lap Joints
Test pieces containing lap joints at their centre in
the as-welded condition shall be selected at the
rate of one sample for tensile test for every 100
joints or as decided by the engineer-in-charge.
13.2.1 Tensile Test
The free specimen length between grips must be
between 25 d and 30 d where d is the nominal
diameter of the bar. The breaking load shall
not be less than the guaranteed load in accor-
dance with IS 1786 : 1985 required to fracture
14.1 If a sample selected for testing fails to meet
the requirements given under 13.1 and 13.2, the
purchaser or his representative shall take two
further samples from the same lot. If on test-
ing, either of the samples fails to meet the
specified requirements, the whole lot shall be
( Chse 2.1 )
LIST OF REFERRED INDIAN STANDARDS
IS No. Title
SP 46 : 1988 Engineering drawing
practice for schools and
IS 812 : 1957 Glossary of terms relat-
ing to welding and cutt-
ing of metals
IS 813 : 1986 Scheme of symbols for
welding ( jirst revision >
IS 814 (iPart 1) : 1974 Specification for cover-
ed electrodes for metal
arc welding of structural
steels : Part 1 For weld-
ing products other than
sheets ( fourth revision )
IS 815 : 1974 Classification and cod-
ing of covered electro-
des for metal arc weld-
ing of structural steels
( second revision )
IS 818 : 1968 Code of practice for
safety and health re-
quirements in electric
and gas welding and
cutting operations ( jirst
IS 1179 : 1967 Specification for equip-
ment for eye and face
protection during weld-
ing ( Jirst revision)
IS 1786 : 1985
1s 1851 : 1975
IS 2635 : 1975
1s 2641 : 1964
IS 2751 : 1979
IS 3016 : 1982
IS 9595 : 1980
IS 9857 : 1981
Specification for high
strengih deformed steel
bars and wires for con-
( third revision )
Specification for single
operator type arc weld-
ing transformers ( se-
cond revision )
Specification for DC
electric welding genera-
tors ( second revision )
Specification for electric
Code of practice for
welding of mild steel
plain and deformed
bars for reinforced con-
crete construction ( Jirst
Code of practice for fire
precautions in welding
and cutting operations
metal arc welding of
carbon and carbon
Specification for weld-
1s 9417 : 1989
( Clause 6.1 )
SELECTION OF EQUIPMENT AND ACCESSORIES FOR WELDING COLD-WORKED
BARS USED FOR REINFORCED CONCRETE CONSTRUCTION
B-l.1 The methods of welding covered in this
a) Flash butt welding, and
b) Shielded metal arc welding with covered
B-2 FLASH BUTT WELDING EQUIPMENT
B-2.1 The efficiency of the flash butt welding
equipment, manifested by its corrjunctive efftcien-
cy for cold-worked steels should be about
8 kVA/cm” of the cross sectional are2 of the bar
in order that sufficient cold weld may be accom-
B-2.2 The jaws for clamping the bars should
preferably be long and pin shaped in order to
assume 2 rectilinear central feeding of the bar
ends. The joint should preferably be of copper
to assume a smooth and uniform flow of current
from the jaws into the bar.
B-3 SHIELDED METAL ARC WELDING
B-3.1 In its simplest form, the equipment
required for shielded metal arc welding of cold-
worked steel bars for concrete reinforcing con-
Welding power source;
Accessories, such as, electrode holders,
earth clamp, welding cable, connectors,
chipping hammer 2nd wire brush;
Protective equipment for the operator,
such as, hand screen or helmet, gloves,
apron, etc; and
Suitable electrode storage and drying
equipment, where necessary.
B-3.1.1 Welding Power Source
The current for welding may be alternating or
direct. There is little to choose between them
for work involving mild steel welding. Electri-
city from the mains is usually at too high 2
voltage for are welding. Various types of equip-
ment are used for reducing this voltage and
delivering 2 welding current of right characteri-
B-220.127.116.11 Alternating current transformer of
oil-cooled or air-cooled type has the advantage
of being low in initial cost and requiring very
little maintenance. Various types of controls
for varying the current to suit conditions are
in common use. Some of these are: (2) a
static choke with tappings, (b) 2 choke the value
of which may be varied by means of the move-
ment of the core, (c) a choke with a saturable
core, and (d) a variable flux linkage transformer.
Being essentially a single-phase load, welding
transformers when connected to 3-phase supply
mains may cause slightly unbalanced load condi-
tions. Condensers of adequate rating may also
be connected across the input lines for improv-
ing the power factor.
B-18.104.22.168 Rotary machines, such as, motor
generators suitable for use on alternating-current
mains give a direct current output of the requir-
ed characteristics. They have the advantage-
that they impose a balanced load on 3-phase
supply mains. They are, however, initially more
expensive and require more maintenance than
B-3.1.2 Where the mains supply is direct current,
a motor generator designed for direct current
mains use has to be selected.
B-3.1.3 Rectifier welding sets which are relative-
ly high in initial cost, require very little main-
tenance because of elimination of most moving
parts. They also impose a balanced load on
3-phase supply. mains.
B-3.1.4 For work at sites where mains power
supply is not available, a petrol or diesel engine
driven welding generator may be selected. Such
machines are often mounted on trailers for easy
B-3.1.5 Other points to be considered when
selecting the equipment are;
that the machine is designed to work satis-
factorily in the climatic conditions that
will be met with during service;
that it is well made and conforms to rele-
vant Indian Standards, wherever these
that the current capacity is adequate for
welding with the sizes of electrodes expect-
ed to be used.
B-22.214.171.124 IS 1851 : 1975 covers transformer
welding equipment and IS 2635 : 1975 covers
motor generator equipment for manual metal arc
B-126.96.36.199 Electrode holders shall conform to the
requirements laid down in IS 2641 : 1964 2nd
shall be of suitable rating for welding with
electrodes in sizes expected to be used.
B-188.8.131.52 Welding cables shall conform to the
requirements laid down in IS 9857 : 1981, if
cables with copper conductors are used. Cables
with aluminium conductors shall be of 2 quality
proved for performance. Two lengths of cables
are required, one from the welding set to the
electrode holder and the other from the work
piece to the welding set.
IS 9417 : 1989
B-184.108.40.206 All cable terminal connections, such
as, sockets-earth clamp, shall also conform to
the requirements specified in IS 2641 : 1964.
B-220.127.116.11 A well made chipping hammer with a
hardened and tough cutting edge and a narrow
type wire brush which may reach the root of the
weld would also be required for deslagging and
cleaning the weld.
B-3.1.6 Protective Equipment
A non-conducting hand screen or helmet fitted
with protective filter lens will be required to
protect the face and eyes of the operator from
the ultra-violet and infra-red rays emitted by
the arc. The filter lens has the double function
of securing good vision of the arc and giving
effective protection by cutting off the harmful
rays. The eye and face protection equipment
should conform to the appropriate stipulations
laid down in IS 1179 : 1967.
B-18.104.22.168 Aprons and leather gloves should be
of a standard that has been proved adequate
for welder’s use. Shoulder guards, leggings and
other such protective garments may be necessary
when the operator has to do positional welding
in conditions where freedom of movement is
The conditions of the electrodes used have an
important bearing on the ultimate quality of
the weld produced. Particularly, when moist
ambient conditions are envisaged, for instance,
at site work, the storage of electrodes has to be
given much attention. Heated storage cabinets
or drying ovens arc a must when low hydrogen
type electrodes are being used for site work.
Other types of electrodes also are preferably
stored before use in such cabinets when ambient
conditions are unfavourable.
( Clause 10.4.2 )
GAS PRESSURE WELDING
C-l GAS PRESSURE WELDING PROCESS
The gas pressure welding process may be used
for butt welding of reinforcing bars.
C-l.1 Preparation for Welding
C-1.1.1 The ends of bars and the extreme un-
twisted ends of new bars shall be cut by shear-
ing or machining to make the face approximately
normal to the axis of the bar. Care should be
taken to ensure that the bar ends do not twist
C-1.1.2 Rust, oil, paint, cement paste and any
other coating over the bar-ends shall be remov-
ed and the surfaces to be welded shall be finish-
ed as flat as possible.
C-1.2.1 Bars are clamped securely in the
clamping unit with no misalignment keeping the
gap between the bar ends less than 3 mm.
C-1.2.2 To begin with, the bar ends are heated
by a reducing flame to avoid any oxide forma-
tion. The flame shall be directed at the joint
and the burner shall be rotated to ensure
uniform heating of the bar ends. On sufficient
heating, the gap between the bar ends shall be
closed by the application of axial pressure
(preliminary or first stage pressurization).
C-1.2.3 After preliminary pressurization and
complete closing of the gap, the bar ends shall
be heated by a neutral flame. The heating shall
be done for an appropriate period ensuring
that the bar ends do not melt.
C-1.2.4 On sufficient heating of the bar ends,
appropriate axial pressure ( final or second
stage pressurization ) is applied so that the
bulge at the weld interface is about 1’4 times
the bar diameter. Heating shall be stopped at
this stage. However, pressure application shall
be maintained for some time even after the
flame is put off.
C-1.2.5 The bars shall be unclamped after the
glow of the heated area vanishes.
C-1.2.6 In case the flame dies out during heat-
ing, the affected area shall be cut off and the
welding procedure begun afresh.
C-2 GAS PRESSURE WELDING
C-2.1 The equipment for gas pressure welding
4 Oxygen and acetylcnc gas cylinders with
regulating values, etc;
b) Multi-nozzle burner;
c>Clamping unit; and
C-2.1.1 The burner consists of a blow pipe with
four or more nozzles. The nozzles shall be so
arranged to ensure uniform heating of the bar
surface. The burner shall provide stable flame
during heating and the heating capacity shall be
appropriate to the size of the bar.
C-2.1.2 The clamping unit shall grip the bars
well, be easy to handle, capable of being used in
horizontal or vertical position of welding, and
have such machanism that no misalignment
develops at the welded portion.
C-2.1.3 Pressurizer shall be either hydraulic or
mechanical and may be either manually operat-
cd or electrically driven. The pressurizer shall
be capable of maintaining uniform axial prcs-
The use of the Standard Mark is governed by the provisions of the Bureau ofthe Indian
Standards, Act, 1986 and the Rules and Regulations made thereunder. The Standard Mark on
products covered by an Indian Standard conveys the assurance that they have been produced
to comply with the requirements of that standard under a well defined system of inspection,
testing and quality control which is devised and supervised by BIS and operated by the pro-
ducer. Standard marked products are also continuously checked by BIS for conformity to
that standard as a further safeguard. Details of conditions under which a licence for the use
of the Standard Mark may be granted to manufacturers or producers may be obtained from
the Bureau of Indian Standards.
B ureau of Indian Standards
BIS is a statutory institution established under the Bureau of Indian Standards Act, I986 to promote
harmonious development of the activities of standardization, marking and quality certification ol
goods and attending to connected matters in the country.
BIS has the copyright of all its publications. No part of these publications may be reproduced in
any form without the prior permission in writing of BIS. This does not preclude the free use, in
the course of implementing the standard, of necessary details, such as symbols and sizes, type or
grade designations. Enquiries relating to copyright be addressed to the Director (Publications), BIS.
Revision of Indian Standards
Indian Standards are reviewed periodically and revised, when necessary and amendments, if any,
are issued from time to time. Users of Indian Standards should ascertain that they are in possession
of the latest amendments or edition. Comments on this Indian Standard may be sent to BIS
giving the following reference :
Dot : No. SMDC 15 ( 2919 )
Amendments Issued Since Publication
Amend No. Date of Issue Text Affected
BUREAU OF INDIAN STANDARDS
Manak Bhavan, 9 Bahadur Shah Zafar Marg, New Delhi 110002
Telephones : 331 01 31, 331 13 75 Telegrams : Manaksanstha
( Common to all Offices )
Regional Offices : Telephone
Manak Bhavan, 9 Bahadur Shah Zafar Marg
NEW DELHI 110002
l/14 C.I.T. Scheme VII M, V.I.P. Road, Maniktola
331 01 31
331 13 75
36 24 99
Northern : SC0 445-446, Sector 35-C, CHANDIGARH 160036 2 18 43
3 16 41
Southern : C.I.T. Campus, 4 Cross Road. MADRAS 600113
Western : Manakalaya, E9 MIDC, Marol, Andheri (East)
Branches : AHMADABAD. BANGALORE. BHOPAL. BHUBANESWAR.
GUWAHATI. HYDERABAD. JAIPUR. KANPUR. PATNA.
fI 1: 2’; ;;
41 29 16
6 32 92 95
Printed at Swatantra Bharat Press, Delhi, India